International Journal of Engineering and Technical Research (IJETR) ISSN: 2321-0869, Volume-2, Issue-10, October 2014
Sol gel Spin Coated ZnO Thin Films for Biosensing Applications Edmund P Samuel, Hemalata Bhadane, Umesh Chandra, D. K. Gautam Abstract—Zinc oxide thin films deposited through sol-gel spin coating method for glucose biosensor applications. The surface morphology of film has been studied through AFM and SEM. Surface morphology investigation clearly reveals the enhancment of the surface area due to porous nature fo the thin films. The increment in surface area leads to a possiblity of improvement of sensitivity through sensing elements. The study has been mainly focused on optimization of annealing temperature and it has been realized that the better crystalline nature of zinc oxide films are obtained at 450 0C. Thin film annealed at 450 0C was found to be having thickness of around 800 Å with refractive index almost 1.86. Index Terms—Zinc Oxide, Glucose Biosensor, Sol-gel
I. INTRODUCTION Biosensors are significant tool in detection and diagnosis of various diseases with ease and efficiently [1, 2]. The electrode made of Zinc oxide (ZnO) loaded with enzymes which are very highly responsive, makes ZnO most remarkably known material for biosensor applications. Particularly, the ZnO nanorods have unique advantages due to high specific surface area, good conductivity, high electron mobility and biocompatibility with the biological molecules . ZnO gained significant attention as it has direct energy band gap of 3.37eV, and most importantly the ZnO thin films can be fabricated using sol-gel technique . The sol-gel technique provides better chemical inertness along with photochemical stability. Through sol-gel one can tune the porosity which is very significant in tailoring the bandgap energy and refractive index of ZnO thin films in accordance to achieve better sensitivity of ZnO based glucose biosensor. ZnO is a very promising material for various applications such as light emitting devices, ultra violet wavelength detection, solar cell with more improved efficiency then polymer based cells, gas sensors etc. [5-8]. Recently, in biosensors, the nanostructured ZnO layers are used due to its, chemical stability, non-toxicity . The Figure 1 shows the schematic representations of the ZnO based biosensors which are having better sensitivity toward biological molecules detection. In the recent years ZnO and MgZnO has been investigated intensively because of their immense potential in biosensor,
Manuscript received October 06, 2014. Edmund Samuel, Material Science and Engineering Department, Jimma University, Jimma, Ethiopia . Hemalata Bhadane, Department of Electronics, North Maharashtra University, Jalgaon, India. Umesh Chandra, Material Science and Engineering Department, Jimma University, Jimma, Ethiopia. D. K. Gautam, Department of Electronics, North Maharashtra University, Jalgaon, India).
light emitting devices, piezoelectric transducers and gas sensors. However, the crystalline structure is the key for achieving the better performance and sensitivity through ZnO thin films. The crystal structure and orientation along with the porosity, highly depends on annealing temperature. Therefore, annealing temperature was considered to be significant for the optimization of ZnO thin film deposition conditions and studied in detailed for its impact over various properties such as refractive index, thickness, surface morphology and crystal orientation. The paper reports thickness and refractive index variation with changes in annealing temperature and the optimized best thin film with its surface morphology and XRD analysis has been included in results and discussion section. The experimental procedure is in section II and the overall discussion of results are presented in section III and finally the conclusion has been presented.
Figure 1 Biosensor structure II. EXPERIMENTAL Zinc Oxide thin films have been deposited by sol-gel spin coating method by using precursor Zinc Acetate dihydrate (Zn(CH3COO)2.2H2O), 2- Methoxyethanol as solvent and Monoethanolamine as the stabilizer. The 0.5M of Zinc acetate (ZnAc) has been dissolved in 2-Methoxyethanol and further monoethanolamine has been added drop wise at room temperature under constant stirring. The concentration of monoethanolamine has been kept 1:1 with the Zinc acetate. This resultant solution has been stirred further at 50°C for 45 min to obtain a homogeneous, clear and transparent solution. The glass substrates have been cleaned with the dilute hydrochloric acid, ethanol and distilled water. The p-type Silicon <100> substrates have been ultrasonically cleaned into acetone and isopropanol in order to remove unwanted
Sol gel Spin Coated ZnO Thin Films for Biosensing Applications
native oxide layer on the wafer surface. Finally, the silicon wafer has been rinsed and cleaned with deionized (DI) water. For the deposition of thin film, the prepared ZnAc transparent solution dropped on the pre cleaned glass substrate and spinning was done with 3000 rpm for 30 sec for uniform deposition of thin film. These deposited ZnO films were preheated at 110°C for 10 min to evaporate any remaining solvent and organic compound. The process of deposition of films and preheating were repeated for ten times to obtain the desired thickness. The films were also deposited on silicon substrate for thickness and refractive index measurement. The prepared thin films were further annealed at the different temperature from 300 to 500 °C using muffle furnace. The thickness and refractive index (RI) were measured by Ellipsometer (Philips SD-1000). The structural property of thin films was studied using the X-ray diffraction (XRD, Rigaku Japan). The surface morphologies and roughness of the spin coated ZnO film was studied using a scanning electron microscope (SEM; JEOL, JSM-6610) and atomic force microscope (AFM; XE-100, Park Systems Corp., Suwon, Korea) respectively.
Figure 2 (b) Effect of annealing temperature on refractive index of films
III. RESULTS AND DISCUSSION Figure 3 XRD pattern of ZnO thin film annealed at 450˚C temperature
Figure 2 (a) Effect of annealing temperature on thickness of films The films deposited on Si substrate were characterized by Ellipsometery for measurement of thickness and refractive index in order to study the effect of annealing temperature as shown in Figure 2(a) & (b).The thickness of films (Fig. 2(a)) are observed to be decreasing from 1080 Å to 725 Å. The lowering in thickness is because of reduction in the hydroxyl groups and other volatile impurities from films due to the annealing. Thus, it can be said that, the annealing significantly removes the water molecules trapped in films. The refractive index has been increased from 1.66 to 1.96. This is due to increase in density of films as well as improved crystallinity. It is observed that the thickness of films is getting lowered with annealing temperature and it is well known that the higher annealing temperature improves crystallinity of films  and reduces the surface area. The higher surface area is more beneficial for sensing application, thus, the optimized temperature in this case is 450˚C. Hence, further, characterization such are XRD, SEM and AFM have been carried out for ZnO thin film annealed at 450 ˚C
The XRD have been used to determine the crystal structure of the ZnO thin film in the range of 20°<2θ<80°. Figure 3 shows the XRD pattern of ZnO thin film annealed at 450°C. It has been seen from the pattern that all major diffraction peaks correspond to the ZnO crystal faces. The diffraction peaks denoted by diamonds ( ♦ ) indicates absence of any preferential orientation that reveals the ZnO film is polycrystalline in nature. The peaks are consistent with the diffraction planes of the hexagonal wurtzite structure of ZnO, as confirmed by JCPDS data card no.36-1451. XRD pattern show six primary peaks at 31.8, 34.49, 36.3, 47.4, 56.6 and 62.8 which can be attributed to the (100), (002), (101), (102), (110) and (103) planes respectively. The average crystal size of film was measured to be ~33 nm using the Debye- Scherrer  formula that also demonstrates nanocrystallinity (<100 nm) in film. The evaluated a and c-axis lattice constants of the film are 0.318 and 0.519 nm respectively, which are slightly smaller than standard values presented in JCPDS 36-1451.
Figure 4 SEM of the ZnO thin film annealed at 450°C. Inset image shows ZnO grains at higher resolution
International Journal of Engineering and Technical Research (IJETR) ISSN: 2321-0869, Volume-2, Issue-10, October 2014 The SEM image presented in Figure 4 shows the morphology of the ZnO thin film. The ganglia-like hills of typical width of about 0.2 µm have been observed in SEM. At higher resolution the grains of ZnO are clearly observed as shown in inset of figure 4. Three dimensional (3D) AFM image of ZnO thin film is presented in Figure 5. Average roughness (Ra) values determined from the XEI data processing analysis software available with the AFM system. The Ra value that is acquired from a 5 µm X 5 µm scanned area of films is 6.4 nm.
with macroscale in appearance”, J. Applied Physics, Vol. 102, 2008, pp. 104305. Han-Yu Shih, Yung-Ting Chen, Chih-Ming Wei,Ming-Hui Chan, Jyong-Kuen Lian, Yang-Fang Chen, and Tai-Yuan Lin “Optical Detection of Glucose Based on a Composite Consisting of Enzymatic ZnO Nanorods and InGaN/GaN Multiple Quantum Wells”,J. Phys. Chem. C, Vol. 115, 2011, pp. 14664. Chi Yang, Chunxiang Xu, and Xuemei Wang, “ZnO/Cu Nanocomposite: A Platform for Direct Electrochemistry of Enzymes and Biosensing Applications”, Langmuir, Vol. 28, 2012, pp.4580. Patil V B, Pawar S G, Patil S L, Krupanidhi S B, “ZnO nanocrystalline thin films: a correlation of microstructural, optoelectronic properties”, Journal of Materials Science: Materials in Electronics, Vol. 21, 2010, pp. 355 Ghule L A, Patil A A, Sapnar K B, Dhole S D, Garadkar K M, “Photocatalytic degradation of methyl orange using ZnO nanorods”, Toxicological & Environmental Chemistry, Vol. 93, 2011, pp. 623.
Dr. Edmund Samuel has completed his Masters and Doctorate in Electronics from North Maharashtra University Jalgaon. He worked as a Research Scientist at IACQER, Nanotechnology Laboratory for Optoelectronics and Biosensor from August 2009 to July 2011. From August 2011 to May 2014 he has been awarded postdoctoral fellowship at Optical Functional Materials Laboratory, Toyota Technological Institute, Nagoya, Japan. Earlier during doctorate he has been awarded the extended senior research fellowship from CSIR, New Delhi. He has research interest and worked on various advanced topics such as Quantum Well, Multiple Quantum Well, Quantum wire and Quantum Dots for different material based heterostructure which includes Nitrides & Oxides. He has also worked for silicon based photonic crystal, tellurite based optical, and ZnO based Biosensor for Glucose detection. Present research work is going on Graphene for CO2 and H2 storage.
Figure 5. 3D AFM image . IV. CONCLUSION The nanocrystalline ZnO thin films are deposited successfully on glass substrates by sol gel spin coating technique. The thickness of ZnO thin films were observed to be decreasing with increase in annealing temperature, however, RI is observed to be increasing. The XRD pattern of ZnO thin film annealed at 450˚C shows polycrystalline wurtzite structure. The AFM and SEM support the porous morphology of film which also suggests increased surface area of films making them useful for biosensing applications. REFERENCES  Saha Shibu, Arya S K, Singh S P, Gupta Vinay, “A novel ZnO-methylene blue nanocomposite matrix for biosensing application” International Journal of Electrochemistry, Vol. 2011, 2011, pp.1.  Mashkoor Ahmad, Caofeng Pan, Zhixiang Luo, and Jing Zhu, “Single ZnO Nanofiber-Based Highly Sensitive Amperometric Glucose Biosensor”, J. Phys. Chem. C, Vol. 114, 2010, pp. 9308.  Yang Zao Ye, Zhizhen Zhao, Binghui Zong Xiaolin, Wang Ping “Synthesis of ZnO nanobundles via Sol–Gel route and application to glucose biosensor”, Journal of Sol-Gel Science and Technology, Vol. 54, 2010, pp. 282.  Raoufi Davood, Raoufi Taha, “The effect of heat treatment on the physical properties of sol–gel derived ZnO thin films”, Applied Surface Science, Vol. 255, 2009, pp. 5812.  Kuchibhatla, Satyanarayana VNT Karakoti, A S Bera, Debasis Seal, S, “One dimensional nanostructured materials”, Progress in materials science, Vol. 52, 2007, pp. 699.  Kim Kwon-Ho, Shin Kyung-Sik, Kumar Brijesh, Kim Kyung-Kook, Kim Sang-Woo, “Mist-CVD growth of high quality ZnO thin films at low temperature for inverted organic solar cells”, Journal of Nanoelectronics and Optoelectronics, Vol. 5, 2010, pp. 247.  Zhang, N Yu, Ke Li, Q Zhu, ZQ Wan, Q, “Room-temperature high-sensitivity HS gas sensor based on dendritic ZnO nanostructures
Hemalata Bhadanae has completed her M.Sc. and M.Phil. in Electronics from Department of Electronics, North Maharashtra University, Jalgaon. She worked as women scientist on DST funded project at IACQER, Nanotechnology Laboratory for Optoelectronics and Biosensor, Raghu Engineering College, Vishakhapatnam for her Ph.D. Her research work is based on simulation of nanostructures and deposition of ZnO thin films by sol gel and electrochemical method. She has published international and national journal papers based on her research and also presented her work in various conferences. Dr. Umesh Chandra He received his MSc and PhD in Industrial Chemistry in 2007 and 2012 respectively from Kuvempu University. He is an assistant professor/postdoctoral researcher in Materials Science and Engineering department, Jimma Institute of Technology, Jimma University, Ethiopia. His research area is electrochemical biosensor. His research interest involves modification of carbon based electrode for electrochemical investigation of several neurotransmitters. He presented his research in various national and international conferences by both oral and poster presentation. He published more than 30 research articles in reputed international journals. Dr D. K. Gautam is Professor at Department of Electronics at North Maharashtra University, Jalgaon and working as a Head since last 20 years. Dr. Gautam started his laboratory from scratch and established a giant centre of high quality research in the field of semiconductor technology which is known nationally and internationally at present for high quality research. He has also started M.Tech in VLSI course via UGC scheme. He has completed sponsored projects of more than Rs. 35 crores from various national and international funding agencies and guided 9 Ph.D. students. He has more than 150 publications and a number of patents to his credit in national and international journals and proceedings of high repute. Dr. Gautam was Director, Board of Colleges and University Development, from 2003 to March 2006 of N.M. University. He has worked as an expert member of several committees of AICTE, UGC, MIT, DST, DBT, and many universities.
Published on Dec 1, 2016